Bar-iron (aka wrought iron) was the raw ingredient for creating a form of steel known commonly as blister steel, and blister steel was in turn the primary ingredient for the “crucible” steel used by Sheffield tool makers.
To convert bar-iron to steel, carbon must be added back into the metal in a controlled fashion. The process used for this was called cementation and the steel produced was therefore also known as cementation steel.
Blister steel – the cementation process
We can learn a little about the history and repute of Leufsta branded iron from a court case heard in 1884: Heaton’s Trademark2)the original court summary can be found in various legal publications from the time including The Law Reports: Cases Determined by the Chancery Division – 1884
The application was opposed by the Baron Louis de Geer, the owner of the Leufsta mine in Dannemora, on the grounds that the hoop L mark was the exclusive property of his firm.
Heaton argued that it was common practice for firms to make their blister steel from cheaper grades of Swedish iron and to then obliterate the original trademark stamp on their cemented-steel bars (the original stamps having survived the cementation process) and replace it with the hoop L stamp so that they could charge more for it. He explained that his firm had been doing it for the past 50 years and that he knew of at least 30 other firms that did exactly the same thing!
Needless to say, the judge threw the trademark application out of court and ordered Heaton to pay costs, summing up with the pithy:
During the court case we learn that the Leufsta hoop L stamp was first registered in Sweden in 1718 and was most likely in use for part of the prior century too. We also learn that the owners granted sole import rights of Leufsta iron to William Jessop and Sons in the 1860s and subsequently to Thomas Firth & Sons from 1880 (prior to 1866 there had been various other importers, including Sykes of Hull).
Here are some contemporary adverts from importers of Leufsta iron:
The Cementation Furnace
The troughs were filled with alternating layers of broken-up charcoal and bar iron and then covered with sand, loam or wheelswarf 3)swarf collected from the troughs of water cooled grindstones –
the swarf was a mixture of water, stone and steel particles from the grinding of edge tools, which caked together as the heat of the furnace increased, sealing the top of the troughs so that air could not enter.
Once the fire was lit the furnace needed about 3 days to get to the temperature where the carbon from the charcoal begins to diffuse into the iron, and from this point it would be kept at temperature for a further 7 to 10 days to allow the process to complete.4)Charles Sanderson, On the Manufacture of Steel, as carried on in this and other Countries; May 9th 1855 ; Journal of the Soc of Arts vol III p454
During this process the carbon would react with impurities in the iron to produce gaseous bubbles that would form the characteristic blisters on the surface of the bar, and this led to the metal being known as ‘blister steel’. 5)as well as ‘blister steel’ and ‘cementation steel’ it was also occasionally referred to as ‘converted’ steel, after the process which was known loosely as ‘conversion’
Once the furnace cooled – a process that could take a further two weeks – the steelmakers would climb into the furnace to break through the layer of material used to seal the troughs (known in Sheffield as crozzle) in order to unpack the bars of converted steel (blister steel was also known generically as ‘bar steel’).
The steel bars were broken at the tip (‘topping’) and the fracture examined so that each bar could be graded according to its ‘temper’ (its degree of carburisation). The bars nearest the fire are more highly carburized than those at the center – in the classification below for the lower numbers the conversion has not passed far into the bar, while the highest number has converted entirely
The steel could be made more homogenous by heating it and subjecting it to the action of a tilt hammer (a hammer capable of striking several hundreds of blows per minute) – this was known as tilt stee.6)p788 The Engineer’s and Mechanic’s Encyclopædia Volume 1 , 1835
A further refined form of blister steel, known as shear steel 7)so called because the inventor – Crowley – was in the habit of stamping his product of a pair of shears to indicate its suitable application, Engineer’s and Mechanics Encylopaedia op. cit. p788, was formed by breaking the thin bars of blister steel to lengths of about 2-4 ft long, and then heating 6 or so strips held together in a bundle.
The red-hot bundle was then placed under a heavy forge hammer which welded the rods together. The thick bar could then be hammered or rolled to the size required (the resulting bar could be doubled up and welded again creating double shear).8)readers based in the UK can see shear and double-shear steel being made in this film, taken Edgar Allen, Sheffield, in 1939:
This subsequent process went some way to making the steel more homogenous but the material still had areas of high and low carbon and this could result in inconsistent hardening. Nonetheless the steel was found to have good qualities for use in the making of razors, knives, swords , shears and scythes.
The image below shows three cementation furnace at Thomas Firth’s Norfolk Works, Sheffield (circa 1900):
A Footnote on German and Puddled Steel
By the turn of the 19th Century the term German Steel seems to be used generically by tool makers (particularly in saw making) to denote any steel deemed to be 2nd quality compared to Sheffield crucible steel, however, the term also describe a steel making technique that was common practice in German steel making regions like Westphalia.
This steel was sometimes referred to as raw or natural steel because it was produced directly from pig iron. 9)c.f Charles Sanderson, ibid, for an account on the different variations used to create steel from pig iron in other countries.
A thin layer of pig iron is melted in a furnace and allowed to stay in the flames until it has partially decarbonized and starts to solidify at which point charcoal is drawn over the top and further pig iron added until it melts, solidifies and combines with the previous layer. This process is repeated until a large enough bloom is created to be withdrawn from the fire and separated into parts.
The amount of carbon retained in the resulting metal was critical to its final quality – too much and it would be brittle, too little and it can’t be hardened – and getting this right depended entirely on the skill of the steelmaker. Even when the carbon content was judged correctly the unrefined steel was nonetheless of limited use for tool making since it was not homogenous, containing some areas with high carbon content, and others with little or none (meaning some parts of a single bar might harden and others not).
This, plus the irregularities in quality from the various makers, meant the steel did not command high prices.
As with blister steel, the metal was improved by forging and welding bars together to make it more homogenous, upon which it was broken and graded according to its ‘temper’ (carbon content).
Refined German steel was was often used in Germany for the making of cutting tools and also put to use in 2nd quality tools in Sheffield, but it was not used for more important purposes and this reflected in the price 10)for instance in 1855 refined German Steel was about half the price of the best blister steel – Sanderson, 1855.
A second technique for producing steel from pig iron was also introduced in Westphalia during the 1st half of the 19th century which involved the use of a puddling furnace. The first step was to puddle (decarbonize) a charge of pig-iron and then to add a second smaller charge of of pig-iron (about 15% of the weight of the original charge) was allowed to melt gradually until it mixed with the metal previously added. The newly introduced carbon rich material caused the original bloom to first boil and then resolidify.
This process retained some of the carbon from the second charge but the resulting steel was rather imperfect and this was reflected in the price – Puddled steel selling even cheaper than unrefined German steel.
References [ + ]
|1.||↑||Charles Sanderson, a sheffield steel maker, in 1855: On the Manufacture of Steel, as carried on in this and other Countries|
|2.||↑||the original court summary can be found in various legal publications from the time including The Law Reports: Cases Determined by the Chancery Division – 1884|
|3.||↑||swarf collected from the troughs of water cooled grindstones –|
the swarf was a mixture of water, stone and steel particles from the grinding of edge tools
|4.||↑||Charles Sanderson, On the Manufacture of Steel, as carried on in this and other Countries; May 9th 1855 ; Journal of the Soc of Arts vol III p454|
|5.||↑||as well as ‘blister steel’ and ‘cementation steel’ it was also occasionally referred to as ‘converted’ steel, after the process which was known loosely as ‘conversion’|
|6.||↑||p788 The Engineer’s and Mechanic’s Encyclopædia Volume 1 , 1835|
|7.||↑||so called because the inventor – Crowley – was in the habit of stamping his product of a pair of shears to indicate its suitable application, Engineer’s and Mechanics Encylopaedia op. cit. p788|
|8.||↑||readers based in the UK can see shear and double-shear steel being made in this film, taken Edgar Allen, Sheffield, in 1939:|
|9.||↑||c.f Charles Sanderson, ibid, for an account on the different variations used to create steel from pig iron in other countries.|
|10.||↑||for instance in 1855 refined German Steel was about half the price of the best blister steel – Sanderson, 1855|